Martensite and Bainite in Steels: Transformation Mechanism ... · PDF file Bainite and...
Embed Size (px)
Transcript of Martensite and Bainite in Steels: Transformation Mechanism ... · PDF file Bainite and...
J PHYS. IV FRANCE 7 ( 1 997) Colloque C5, SupplCment au Journal de Physique I11 de novembre 1997
Martensite and Bainite in Steels: Transformation Mechanism & Mechanical Properties
University of Cambridge, Materials Science and Metallurgy, Pembroke Street, Cambridge CB2 3Q.Z U. K.
Abstract: Many essential properties of iron alloys depend on what actually happens when one allotropic form gives way to another, i.e. on the mechanism of phase change. The dependence 05 the$ mechanical properties on the atomic mechanism by which bainite and martensite grow is the focus of this paper. The discussion is illustrated in the context of some common engineering design parameters, and with a brief example of the inverse problem in which the mechanism may be a function of the mechanical properties.
1. INTRODUCTION More than 70% of all the steel that is used in modern economies has been invented within the last ten years. Novel iron alloys are being conceived, manufactured and marketed with a regularity which has confounded many prophecies. There is also elation in academia, because a few of the interesting alloys have come about from a basic understanding of steels.
The science is usually in the form of the detailed mechanisms of phase transformations, but this alone cannot lead to better steels. I t is the mechanical properties which are important to engineers, who generally do not have a passion for transformations. To them, design does not consist simply of some theoretical calculations which produce an alloy with the required properties. The manufacture of any new material must be at a competitive cost, and it ought to be possible to fabricate it without difficulty. The new development may necessitate additional or novel manufacturing equipment. The best steel companies only permit capital investment if the profit is improved sufficiently to pay off that investment within two years. This is because the steel industry has in the past focussed too heavily on fixed assets with large burdens of debt servicing. On the other hand, the discovery may, in rare circumstances, be of sufficient importance to warrant longer term strategic investment.
It is worth emphasizing that good design usually emerges from a problem which does not have a unique solution. Creativity is therefore as important as scientific design in the commercial success of an alloy. It is frequently useful to design more than one alloy (or microstructure or heat treatment) for the same purpose. It is in this light that we shall consider the relationship between the mechanism and mechanical properties of two microstructures rather than one. For the sake of economy. we shall assume that the basic experimental features of both bainite and martensite are well known. for example, the plate shape, the shape deformation, the role of the alloying elements etc.
2. MECHANISM OF DISPLACIVE TRANSFORMATION The Bain strain converts the structure of the parent phase into that of the product phase. When combined with an appropriate rigid body rotation, the net homogeneous lattice deformation RB is an invariant-line strain (Fig. l ) , giving good fit only along a single line common to the two crystals. However, the observed shape deformation indicates a larger degree of fit. The shape change is in fact an invariant-plane strain (IPS) P,, but this gives the wrong crystal structure. If, however, a second homogeneous shear Pg is combined with PI, then the correct structure is obtained but the wrong shape since
Article published online by EDP Sciences and available at http://dx.doi.org/10.1051/jp4:1997558
C5-368 JOURNAL DE PHYSIQUE IV
These discrepancies are all resolved if the shape changing effect of P, is canceled macroscopically by an inhomogeneous lattice-invariant deformation, which may be slip or twinning as illustrated in Fig. 1.
The theory illustrated explains all the essential features of martensite or bainite crystallography [1,2]. It is easy to predict the orientation relationship, by deducing the Bain strain and adding a rigid body rotation which makes the net lattice deformation an invariant-line strain. The habit plane does not have rational indices because the amount of lattice-invariant deformation needed to recover the correct macroscopic shape is not usually rational. The theory predicts a substructure in plates of martensite (either twins or slip steps) as is observed experimentally. The transformation goes to all the trouble of ensuring that the shape deformation is macroscopically an invariant-plane strain because this reduces the strain energy when compared with the case where the shape deformation might be an invariant-line strain.
-INVARIANT DEFORMATION /' I """
Twinned Slipped Martensite Martensite
Correct rnacroscop>c shape, correct structure
Fig. 1: Illustration of the phenomenological theory of martensite crystallography .
The mechanism of transformation outlined above is valid for both martensitic and bainitic transfor- mations, though there are subtle differences. It is not appropriate here to discuss these in detail, but some of important characteristics are highlighted in Table 1. We shall now proceed to relate mechanical properties to the mechanism of transformation.
Table 1: Ransformation characteristics for bainite (ab) and martensite (a') (41.
Nucleation & growth reaction J J
Plate shape J J Diffusionless nucleation J x
Carbon diffusion during nucleation x J
Substitutional diffusion during nucleation X x
Confined to austenite grain J
3. TEMPER EMBRITTLEMENT The observed IPS shape deformation during displacive transformation in steel proves that there is a synchronized motion of atoms. Such a coordinated motion of atoms cannot be sustained across austenite
Large shear J J IPS shape deformation J J Diffusionless growth J d Carbon diffusion during growth x x
Substitutional diffusion during growth x x
Glissile interface J J
grain boundaries. Bainite and martensite plates are therefore confined within the grain in which they nucleate. This is not the case for reconstructive transformations in which all the atoms diffuse. Thus, allotriomorphic ferrite and pearlite can grow freely across austenite grain boundaries, thereby removing them from the microstructure.
On the other hand, with displacive transformations, a vestige of the austenite grain boundary remains even in a fully transformed microstructure. The misfit present a t the original austenite grain boundaries can evidently be inherited in a fully transformed specimen. This is because the displacive transformation of austenite involves a minimal movement of atoms. The Bain Strain, which is the pure component of the deformation which converts the austenite lattice into that of ferrite, does not rotate any plane or direction by more than about 11' . And the change in volume during transformation is a mere few percent.
The prior austenite grain boundaries in martensitic or bainitic steels therefore represent regions of atomic disorder in the original y/y boundaries, which are highly susceptible to the segregation of impurity atoms such as phosphorus .
Martensitic and bainitic steels are therefore particularly prone to temper embrittlement phenomena , to embrittlement by liquid zinc  and to failure by creep defects a t the prior boundaries .
4. QUANTITATIVE FRACTURE TOUGHNESS Much of the literature about toughness tends to focus on micromechanisms, test methodology or pro- cedures for using experimental data in design excercises. By contrast, there is very little work on the predzctzon of the energy absorbed during fracture. This difficulty is illustrated by some basic concepts of fracture mechanics. The critical value Klc of the stress intensity which must be exceeded to induce rapid crack propagation is the product of two terms
KIc = stress x distance4 (2)
where the stress is a fracture stress oF which can measured independently using notched tensile specimens. It can be related to the microstructure via [10,11]:
where E is the Young's modulus and v is the Poisson's ratio. yp is the effective work done in creating a unit area of crack plane, estimated to be about 14 J m P 2 for many iron-base microstructures ; it is much larger than a surface energy (typically 1 J m-') because of the plastic zone which moves with the crack tip. This value of 14 J mP2 seems t o apply to a wide variety of steel microstructures . which is surprising given that they often have quite different deformation characteristics. In any event, there is no obvious way of relating yp to the details of the microstructure. By contrast, the dimension c is usually attributed t o the size of a sharp crack created by the fracture of a brittle microstructural constituent such as a cementite particle or a non-metallic inclusion.
. . I. ; , . ; I !
: \ i . I ; ' . ', :.. \ : 3 ::
0.2% proof stress / MPa
Fig. 2: Fracture toughness KIc as a function of the strength 
C5-370 JOURNAL DE PHYSIQUE IV
The other parameter in equation 2, distance;, refers to a length ahead of the crack tip, within which the stress is large enough to cause the fracture of brittle crack-initiators.
We can now examine the observed fracture toughness behaviour for engineering steels with bainitic or marte